#------------------------------------------------------------------------------
#$Date: 2021-05-16 12:36:21 +0300 (Sun, 16 May 2021) $
#$Revision: 265253 $
#$URL: file:///home/coder/svn-repositories/cod/cif/4/00/08/4000836.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4000836
loop_
_publ_author_name
'Huang, Hongwei'
'Yao, Jiyong'
'Lin, Zheshuai'
'Wang, Xiaoyang'
'He, Ran'
'Yao, Wenjiao'
'Zhai, Naixia'
'Chen, Chuangtian'
_publ_section_title
;
 Molecular Engineering Design to Resolve the Layering Habit and
 Polymorphism Problems in Deep UV NLO Crystals: New Structures in
 MM′Be2B2O6F (M═Na, M′═Ca; M═ K,
 M′═Ca, Sr)
;
_journal_issue                   24
_journal_name_full               'Chemistry of Materials'
_journal_page_first              5457
_journal_paper_doi               10.1021/cm202870q
_journal_volume                  23
_journal_year                    2011
_chemical_formula_sum            'B2 Be2 Ca F K O6'
_chemical_formula_weight         233.82
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           163
_symmetry_space_group_name_Hall  '-P 3 2c'
_symmetry_space_group_name_H-M   'P -3 1 c'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                120.00
_cell_formula_units_Z            2
_cell_length_a                   4.7054(16)
_cell_length_b                   4.7054(16)
_cell_length_c                   14.554(3)
_cell_measurement_temperature    293(2)
_cell_volume                     279.07(15)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0252
_diffrn_reflns_av_sigmaI/netI    0.0111
_diffrn_reflns_limit_h_max       6
_diffrn_reflns_limit_h_min       -6
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -20
_diffrn_reflns_number            3409
_diffrn_reflns_theta_full        29.98
_diffrn_reflns_theta_max         29.98
_diffrn_reflns_theta_min         5.00
_exptl_absorpt_coefficient_mu    1.869
_exptl_crystal_density_diffrn    2.783
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             228
_refine_diff_density_max         0.265
_refine_diff_density_min         -0.406
_refine_diff_density_rms         0.077
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.090
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     22
_refine_ls_number_reflns         283
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.090
_refine_ls_R_factor_all          0.0215
_refine_ls_R_factor_gt           0.0193
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0500P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0666
_refine_ls_wR_factor_ref         0.0688
_reflns_number_gt                267
_reflns_number_total             283
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            cm202870q_si_002.cif
_cod_data_source_block           final
_cod_depositor_comments
;

2021-05-16
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_sum            'B4 Be4 Ca2 F2 K2 O12'
_cod_original_formula_weight         467.64
_cod_original_formula_units_Z            1
_cod_database_code               4000836
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-y, -x, -z+1/2'
'x, x-y, -z+1/2'
'-x+y, y, -z+1/2'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
'y, x, z-1/2'
'-x, -x+y, z-1/2'
'x-y, -y, z-1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ca1 Ca -1.0000 0.0000 0.0000 0.0047(2) Uani 1 6 d S
K1 K -1.0000 0.0000 -0.2500 0.0063(2) Uani 1 6 d S
Be1 Be -1.6667 -0.3333 -0.13343(17) 0.0058(5) Uani 1 3 d S
B4 B -0.3333 0.3333 -0.10578(15) 0.0048(4) Uani 1 3 d S
O1 O -1.3756(2) -0.3978(2) -0.10443(6) 0.0059(2) Uani 1 1 d .
F1 F -0.3333 0.3333 0.2500 0.0082(4) Uani 1 6 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
B B 0.0013 0.0007 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Be Be 0.0005 0.0002 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ca Ca 0.2262 0.3064 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
F F 0.0171 0.0103 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O1 Ca1 O1 180.00(3) 7_355 .
O1 Ca1 O1 96.64(3) 7_355 3_345
O1 Ca1 O1 83.36(3) . 3_345
O1 Ca1 O1 83.36(3) 7_355 9_565
O1 Ca1 O1 96.64(3) . 9_565
O1 Ca1 O1 180.00(3) 3_345 9_565
O1 Ca1 O1 83.36(3) 7_355 8_445
O1 Ca1 O1 96.64(3) . 8_445
O1 Ca1 O1 96.64(3) 3_345 8_445
O1 Ca1 O1 83.36(3) 9_565 8_445
O1 Ca1 O1 96.64(3) 7_355 2_465
O1 Ca1 O1 83.36(3) . 2_465
O1 Ca1 O1 83.36(3) 3_345 2_465
O1 Ca1 O1 96.64(3) 9_565 2_465
O1 Ca1 O1 180.00(5) 8_445 2_465
O1 Ca1 B4 106.42(3) 7_355 1_455
O1 Ca1 B4 73.58(3) . 1_455
O1 Ca1 B4 24.46(2) 3_345 1_455
O1 Ca1 B4 155.54(2) 9_565 1_455
O1 Ca1 B4 75.79(4) 8_445 1_455
O1 Ca1 B4 104.21(4) 2_465 1_455
O1 Ca1 B4 24.46(3) 7_355 7_465
O1 Ca1 B4 155.54(3) . 7_465
O1 Ca1 B4 75.79(4) 3_345 7_465
O1 Ca1 B4 104.21(4) 9_565 7_465
O1 Ca1 B4 73.58(3) 8_445 7_465
O1 Ca1 B4 106.42(3) 2_465 7_465
B4 Ca1 B4 82.22(5) 1_455 7_465
O1 Ca1 B4 73.58(3) 7_355 7_455
O1 Ca1 B4 106.42(3) . 7_455
O1 Ca1 B4 155.54(3) 3_345 7_455
O1 Ca1 B4 24.46(2) 9_565 7_455
O1 Ca1 B4 104.21(4) 8_445 7_455
O1 Ca1 B4 75.79(4) 2_465 7_455
B4 Ca1 B4 180.00(7) 1_455 7_455
B4 Ca1 B4 97.78(5) 7_465 7_455
O1 Ca1 B4 155.54(3) 7_355 1_445
O1 Ca1 B4 24.46(3) . 1_445
O1 Ca1 B4 104.21(4) 3_345 1_445
O1 Ca1 B4 75.79(4) 9_565 1_445
O1 Ca1 B4 106.42(3) 8_445 1_445
O1 Ca1 B4 73.58(3) 2_465 1_445
B4 Ca1 B4 97.78(5) 1_455 1_445
B4 Ca1 B4 180.00(7) 7_465 1_445
B4 Ca1 B4 82.22(5) 7_455 1_445
O1 Ca1 B4 75.79(4) 7_355 .
O1 Ca1 B4 104.21(4) . .
O1 Ca1 B4 73.58(3) 3_345 .
O1 Ca1 B4 106.42(3) 9_565 .
O1 Ca1 B4 155.54(3) 8_445 .
O1 Ca1 B4 24.46(3) 2_465 .
B4 Ca1 B4 97.78(5) 1_455 .
B4 Ca1 B4 82.22(5) 7_465 .
B4 Ca1 B4 82.22(5) 7_455 .
B4 Ca1 B4 97.78(5) 1_445 .
O1 Ca1 B4 104.21(4) 7_355 7_355
O1 Ca1 B4 75.79(4) . 7_355
O1 Ca1 B4 106.42(3) 3_345 7_355
O1 Ca1 B4 73.58(3) 9_565 7_355
O1 Ca1 B4 24.46(3) 8_445 7_355
O1 Ca1 B4 155.54(3) 2_465 7_355
B4 Ca1 B4 82.22(5) 1_455 7_355
B4 Ca1 B4 97.78(5) 7_465 7_355
B4 Ca1 B4 97.78(5) 7_455 7_355
B4 Ca1 B4 82.22(5) 1_445 7_355
B4 Ca1 B4 180.00(7) . 7_355
F1 K1 F1 120.0 7_455 7_465
F1 K1 F1 120.0 7_455 7_355
F1 K1 F1 120.0 7_465 7_355
F1 K1 O1 125.458(19) 7_455 3_345
F1 K1 O1 56.786(19) 7_465 3_345
F1 K1 O1 88.147(14) 7_355 3_345
F1 K1 O1 125.458(19) 7_455 5_564
F1 K1 O1 88.147(14) 7_465 5_564
F1 K1 O1 56.786(19) 7_355 5_564
O1 K1 O1 109.08(4) 3_345 5_564
F1 K1 O1 56.786(19) 7_455 2_465
F1 K1 O1 88.147(14) 7_465 2_465
F1 K1 O1 125.458(19) 7_355 2_465
O1 K1 O1 68.75(3) 3_345 2_465
O1 K1 O1 176.29(3) 5_564 2_465
F1 K1 O1 56.786(19) 7_455 6_354
F1 K1 O1 125.458(19) 7_465 6_354
F1 K1 O1 88.147(14) 7_355 6_354
O1 K1 O1 176.29(3) 3_345 6_354
O1 K1 O1 68.75(3) 5_564 6_354
O1 K1 O1 113.57(4) 2_465 6_354
F1 K1 O1 88.147(14) 7_455 .
F1 K1 O1 125.458(19) 7_465 .
F1 K1 O1 56.786(19) 7_355 .
O1 K1 O1 68.75(3) 3_345 .
O1 K1 O1 113.57(4) 5_564 .
O1 K1 O1 68.75(3) 2_465 .
O1 K1 O1 109.08(4) 6_354 .
F1 K1 O1 88.147(14) 7_455 4_444
F1 K1 O1 56.786(19) 7_465 4_444
F1 K1 O1 125.458(19) 7_355 4_444
O1 K1 O1 113.57(4) 3_345 4_444
O1 K1 O1 68.75(3) 5_564 4_444
O1 K1 O1 109.08(4) 2_465 4_444
O1 K1 O1 68.75(3) 6_354 4_444
O1 K1 O1 176.29(3) . 4_444
F1 K1 Be1 115.094(11) 7_455 1_665
F1 K1 Be1 31.98(4) 7_465 1_665
F1 K1 Be1 115.094(11) 7_355 1_665
O1 K1 Be1 29.98(3) 3_345 1_665
O1 K1 Be1 111.97(3) 5_564 1_665
O1 K1 Be1 64.59(3) 2_465 1_665
O1 K1 Be1 153.34(3) 6_354 1_665
O1 K1 Be1 95.19(4) . 1_665
O1 K1 Be1 86.39(4) 4_444 1_665
F1 K1 Be1 115.094(11) 7_455 4_334
F1 K1 Be1 115.094(11) 7_465 4_334
F1 K1 Be1 31.98(4) 7_355 4_334
O1 K1 Be1 111.97(3) 3_345 4_334
O1 K1 Be1 29.98(3) 5_564 4_334
O1 K1 Be1 153.34(3) 2_465 4_334
O1 K1 Be1 64.59(3) 6_354 4_334
O1 K1 Be1 86.39(4) . 4_334
O1 K1 Be1 95.19(4) 4_444 4_334
Be1 K1 Be1 129.81(2) 1_665 4_334
F1 K1 Be1 31.98(4) 7_455 4_434
F1 K1 Be1 115.094(11) 7_465 4_434
F1 K1 Be1 115.093(11) 7_355 4_434
O1 K1 Be1 153.34(3) 3_345 4_434
O1 K1 Be1 95.19(4) 5_564 4_434
O1 K1 Be1 86.39(4) 2_465 4_434
O1 K1 Be1 29.98(3) 6_354 4_434
O1 K1 Be1 111.97(3) . 4_434
O1 K1 Be1 64.59(3) 4_444 4_434
Be1 K1 Be1 129.81(2) 1_665 4_434
Be1 K1 Be1 94.54(5) 4_334 4_434
O1 Be1 O1 113.31(7) 2_365 3_235
O1 Be1 O1 113.30(7) 2_365 .
O1 Be1 O1 113.30(7) 3_235 .
O1 Be1 F1 105.29(9) 2_365 7_355
O1 Be1 F1 105.29(9) 3_235 7_355
O1 Be1 F1 105.29(9) . 7_355
O1 Be1 K1 60.73(5) 2_365 1_455
O1 Be1 K1 90.03(5) 3_235 1_455
O1 Be1 K1 155.17(9) . 1_455
F1 Be1 K1 58.02(4) 7_355 1_455
O1 Be1 K1 155.17(9) 2_365 1_445
O1 Be1 K1 60.73(5) 3_235 1_445
O1 Be1 K1 90.03(4) . 1_445
F1 Be1 K1 58.02(4) 7_355 1_445
K1 Be1 K1 94.54(5) 1_455 1_445
O1 Be1 K1 90.03(5) 2_365 .
O1 Be1 K1 155.17(9) 3_235 .
O1 Be1 K1 60.73(5) . .
F1 Be1 K1 58.02(4) 7_355 .
K1 Be1 K1 94.54(5) 1_455 .
K1 Be1 K1 94.54(5) 1_445 .
O1 Be1 Ca1 40.86(5) 2_365 1_455
O1 Be1 Ca1 73.33(6) 3_235 1_455
O1 Be1 Ca1 125.66(11) . 1_455
F1 Be1 Ca1 125.56(4) 7_355 1_455
K1 Be1 Ca1 67.54(2) 1_455 1_455
K1 Be1 Ca1 130.771(8) 1_445 1_455
K1 Be1 Ca1 130.771(8) . 1_455
O1 Be1 Ca1 73.33(6) 2_365 .
O1 Be1 Ca1 125.66(11) 3_235 .
O1 Be1 Ca1 40.86(5) . .
F1 Be1 Ca1 125.56(4) 7_355 .
K1 Be1 Ca1 130.771(8) 1_455 .
K1 Be1 Ca1 130.771(8) 1_445 .
K1 Be1 Ca1 67.54(2) . .
Ca1 Be1 Ca1 89.58(5) 1_455 .
O1 Be1 Ca1 125.66(11) 2_365 1_445
O1 Be1 Ca1 40.86(5) 3_235 1_445
O1 Be1 Ca1 73.33(6) . 1_445
F1 Be1 Ca1 125.56(4) 7_355 1_445
K1 Be1 Ca1 130.771(8) 1_455 1_445
K1 Be1 Ca1 67.54(2) 1_445 1_445
K1 Be1 Ca1 130.771(8) . 1_445
Ca1 Be1 Ca1 89.58(5) 1_455 1_445
Ca1 Be1 Ca1 89.58(5) . 1_445
O1 B4 O1 119.979(5) 3_445 2_465
O1 B4 O1 119.980(5) 3_445 1_665
O1 B4 O1 119.980(5) 2_465 1_665
O1 B4 Ca1 83.34(6) 3_445 1_665
O1 B4 Ca1 142.64(11) 2_465 1_665
O1 B4 Ca1 45.57(6) 1_665 1_665
O1 B4 Ca1 45.57(6) 3_445 1_655
O1 B4 Ca1 83.34(6) 2_465 1_655
O1 B4 Ca1 142.64(11) 1_665 1_655
Ca1 B4 Ca1 97.78(5) 1_665 1_655
O1 B4 Ca1 142.64(11) 3_445 .
O1 B4 Ca1 45.57(6) 2_465 .
O1 B4 Ca1 83.34(6) 1_665 .
Ca1 B4 Ca1 97.78(5) 1_665 .
Ca1 B4 Ca1 97.78(5) 1_655 .
O1 B4 K1 137.58(11) 3_445 .
O1 B4 K1 51.57(6) 2_465 .
O1 B4 K1 84.82(6) 1_665 .
Ca1 B4 K1 130.216(12) 1_665 .
Ca1 B4 K1 130.216(12) 1_655 .
Ca1 B4 K1 67.23(2) . .
O1 B4 K1 51.57(6) 3_445 1_655
O1 B4 K1 84.82(6) 2_465 1_655
O1 B4 K1 137.58(11) 1_665 1_655
Ca1 B4 K1 130.216(12) 1_665 1_655
Ca1 B4 K1 67.23(2) 1_655 1_655
Ca1 B4 K1 130.216(12) . 1_655
K1 B4 K1 86.52(5) . 1_655
O1 B4 K1 84.82(6) 3_445 1_665
O1 B4 K1 137.58(11) 2_465 1_665
O1 B4 K1 51.57(6) 1_665 1_665
Ca1 B4 K1 67.23(2) 1_665 1_665
Ca1 B4 K1 130.216(12) 1_655 1_665
Ca1 B4 K1 130.216(12) . 1_665
K1 B4 K1 86.52(5) . 1_665
K1 B4 K1 86.52(5) 1_655 1_665
B4 O1 Be1 134.54(7) 1_445 .
B4 O1 Ca1 109.97(7) 1_445 .
Be1 O1 Ca1 112.96(6) . .
B4 O1 K1 105.74(8) 1_445 .
Be1 O1 K1 89.29(7) . .
Ca1 O1 K1 89.15(4) . .
Be1 F1 Be1 180.0 7_355 10_576
Be1 F1 K1 90.0 7_355 7_455
Be1 F1 K1 90.0 10_576 7_455
Be1 F1 K1 90.0 7_355 7_465
Be1 F1 K1 90.0 10_576 7_465
K1 F1 K1 120.0 7_455 7_465
Be1 F1 K1 90.0 7_355 7_355
Be1 F1 K1 90.0 10_576 7_355
K1 F1 K1 120.0 7_455 7_355
K1 F1 K1 120.0 7_465 7_355
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ca1 O1 2.3725(10) 7_355
Ca1 O1 2.3725(10) .
Ca1 O1 2.3725(10) 3_345
Ca1 O1 2.3725(10) 9_565
Ca1 O1 2.3725(10) 8_445
Ca1 O1 2.3725(10) 2_465
Ca1 B4 3.1226(14) 1_455
Ca1 B4 3.1226(14) 7_465
Ca1 B4 3.1226(14) 7_455
Ca1 B4 3.1226(14) 1_445
Ca1 B4 3.1226(14) .
Ca1 B4 3.1226(14) 7_355
K1 F1 2.7167(9) 7_455
K1 F1 2.7167(9) 7_465
K1 F1 2.7167(9) 7_355
K1 O1 2.7942(10) 3_345
K1 O1 2.7942(10) 5_564
K1 O1 2.7942(10) 2_465
K1 O1 2.7942(10) 6_354
K1 O1 2.7942(10) .
K1 O1 2.7942(10) 4_444
K1 Be1 3.2029(15) 1_665
K1 Be1 3.2029(15) 4_334
K1 Be1 3.2029(15) 4_434
Be1 O1 1.6004(11) 2_365
Be1 O1 1.6004(11) 3_235
Be1 O1 1.6004(11) .
Be1 F1 1.697(2) 7_355
Be1 K1 3.2029(15) 1_455
Be1 K1 3.2029(15) 1_445
Be1 Ca1 3.3394(16) 1_455
Be1 Ca1 3.3394(16) 1_445
B4 O1 1.3757(8) 3_445
B4 O1 1.3757(8) 2_465
B4 O1 1.3757(8) 1_665
B4 Ca1 3.1226(14) 1_665
B4 Ca1 3.1226(14) 1_655
B4 K1 3.4330(16) 1_655
B4 K1 3.4330(16) 1_665
O1 B4 1.3757(8) 1_445
F1 Be1 1.697(2) 7_355
F1 Be1 1.697(2) 10_576
F1 K1 2.7167(9) 7_455
F1 K1 2.7167(9) 7_465
F1 K1 2.7167(9) 7_355
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_4
F1 K1 Be1 O1 144.90(6) 7_455 2_365
F1 K1 Be1 O1 -1.09(9) 7_465 2_365
F1 K1 Be1 O1 -108.10(8) 7_355 2_365
O1 K1 Be1 O1 25.77(7) 3_345 2_365
O1 K1 Be1 O1 -87.35(8) 5_564 2_365
O1 K1 Be1 O1 89.29(8) 2_465 2_365
O1 K1 Be1 O1 -152.70(7) 6_354 2_365
O1 K1 Be1 O1 116.95(12) . 2_365
O1 K1 Be1 O1 -66.56(13) 4_444 2_365
Be1 K1 Be1 O1 24.44(10) 1_665 2_365
Be1 K1 Be1 O1 -108.10(8) 4_334 2_365
Be1 K1 Be1 O1 178.91(9) 4_434 2_365
F1 K1 Be1 O1 -54.5(2) 7_455 3_235
F1 K1 Be1 O1 159.5(2) 7_465 3_235
F1 K1 Be1 O1 52.5(2) 7_355 3_235
O1 K1 Be1 O1 -173.6(2) 3_345 3_235
O1 K1 Be1 O1 73.2(2) 5_564 3_235
O1 K1 Be1 O1 -110.1(2) 2_465 3_235
O1 K1 Be1 O1 7.9(2) 6_354 3_235
O1 K1 Be1 O1 -82.46(16) . 3_235
O1 K1 Be1 O1 94.03(16) 4_444 3_235
Be1 K1 Be1 O1 -174.98(18) 1_665 3_235
Be1 K1 Be1 O1 52.5(2) 4_334 3_235
Be1 K1 Be1 O1 -20.5(2) 4_434 3_235
F1 K1 Be1 O1 27.95(7) 7_455 .
F1 K1 Be1 O1 -118.04(5) 7_465 .
F1 K1 Be1 O1 134.95(6) 7_355 .
O1 K1 Be1 O1 -91.18(8) 3_345 .
O1 K1 Be1 O1 155.70(5) 5_564 .
O1 K1 Be1 O1 -27.66(5) 2_465 .
O1 K1 Be1 O1 90.35(8) 6_354 .
O1 K1 Be1 O1 176.49(3) 4_444 .
Be1 K1 Be1 O1 -92.51(4) 1_665 .
Be1 K1 Be1 O1 134.95(6) 4_334 .
Be1 K1 Be1 O1 61.96(5) 4_434 .
F1 K1 Be1 F1 -107.004(17) 7_455 7_355
F1 K1 Be1 F1 107.004(17) 7_465 7_355
O1 K1 Be1 F1 133.87(2) 3_345 7_355
O1 K1 Be1 F1 20.750(16) 5_564 7_355
O1 K1 Be1 F1 -162.614(15) 2_465 7_355
O1 K1 Be1 F1 -44.60(2) 6_354 7_355
O1 K1 Be1 F1 -134.95(6) . 7_355
O1 K1 Be1 F1 41.54(6) 4_444 7_355
Be1 K1 Be1 F1 132.53(3) 1_665 7_355
Be1 K1 Be1 F1 0.0 4_334 7_355
Be1 K1 Be1 F1 -72.996(17) 4_434 7_355
F1 K1 Be1 K1 -154.470(13) 7_455 1_455
F1 K1 Be1 K1 59.54(5) 7_465 1_455
F1 K1 Be1 K1 -47.47(3) 7_355 1_455
O1 K1 Be1 K1 86.41(3) 3_345 1_455
O1 K1 Be1 K1 -26.72(3) 5_564 1_455
O1 K1 Be1 K1 149.92(3) 2_465 1_455
O1 K1 Be1 K1 -92.07(3) 6_354 1_455
O1 K1 Be1 K1 177.58(8) . 1_455
O1 K1 Be1 K1 -5.92(9) 4_444 1_455
Be1 K1 Be1 K1 85.07(6) 1_665 1_455
Be1 K1 Be1 K1 -47.47(3) 4_334 1_455
Be1 K1 Be1 K1 -120.46(5) 4_434 1_455
F1 K1 Be1 K1 -59.54(5) 7_455 1_445
F1 K1 Be1 K1 154.470(13) 7_465 1_445
F1 K1 Be1 K1 47.47(3) 7_355 1_445
O1 K1 Be1 K1 -178.66(5) 3_345 1_445
O1 K1 Be1 K1 68.22(4) 5_564 1_445
O1 K1 Be1 K1 -115.15(3) 2_465 1_445
O1 K1 Be1 K1 2.86(4) 6_354 1_445
O1 K1 Be1 K1 -87.49(4) . 1_445
O1 K1 Be1 K1 89.01(5) 4_444 1_445
Be1 K1 Be1 K1 180.0 1_665 1_445
Be1 K1 Be1 K1 47.47(3) 4_334 1_445
Be1 K1 Be1 K1 -25.530(13) 4_434 1_445
F1 K1 Be1 Ca1 141.48(6) 7_455 1_455
F1 K1 Be1 Ca1 -4.52(9) 7_465 1_455
F1 K1 Be1 Ca1 -111.52(7) 7_355 1_455
O1 K1 Be1 Ca1 22.35(6) 3_345 1_455
O1 K1 Be1 Ca1 -90.77(7) 5_564 1_455
O1 K1 Be1 Ca1 85.87(8) 2_465 1_455
O1 K1 Be1 Ca1 -156.12(6) 6_354 1_455
O1 K1 Be1 Ca1 113.53(12) . 1_455
O1 K1 Be1 Ca1 -69.98(13) 4_444 1_455
Be1 K1 Be1 Ca1 21.01(10) 1_665 1_455
Be1 K1 Be1 Ca1 -111.52(7) 4_334 1_455
Be1 K1 Be1 Ca1 175.48(9) 4_434 1_455
F1 K1 Be1 Ca1 72.996(17) 7_455 .
F1 K1 Be1 Ca1 -72.996(17) 7_465 .
F1 K1 Be1 Ca1 180.0 7_355 .
O1 K1 Be1 Ca1 -46.13(2) 3_345 .
O1 K1 Be1 Ca1 -159.250(16) 5_564 .
O1 K1 Be1 Ca1 17.386(16) 2_465 .
O1 K1 Be1 Ca1 135.40(2) 6_354 .
O1 K1 Be1 Ca1 45.05(6) . .
O1 K1 Be1 Ca1 -138.46(6) 4_444 .
Be1 K1 Be1 Ca1 -47.47(3) 1_665 .
Be1 K1 Be1 Ca1 180.0 4_334 .
Be1 K1 Be1 Ca1 107.004(17) 4_434 .
F1 K1 Be1 Ca1 4.52(9) 7_455 1_445
F1 K1 Be1 Ca1 -141.48(6) 7_465 1_445
F1 K1 Be1 Ca1 111.52(7) 7_355 1_445
O1 K1 Be1 Ca1 -114.61(9) 3_345 1_445
O1 K1 Be1 Ca1 132.27(8) 5_564 1_445
O1 K1 Be1 Ca1 -51.09(7) 2_465 1_445
O1 K1 Be1 Ca1 66.92(9) 6_354 1_445
O1 K1 Be1 Ca1 -23.43(5) . 1_445
O1 K1 Be1 Ca1 153.06(5) 4_444 1_445
Be1 K1 Be1 Ca1 -115.95(5) 1_665 1_445
Be1 K1 Be1 Ca1 111.52(7) 4_334 1_445
Be1 K1 Be1 Ca1 38.52(6) 4_434 1_445
O1 Ca1 Be1 O1 12.17(14) 7_355 2_365
O1 Ca1 Be1 O1 -167.83(14) . 2_365
O1 Ca1 Be1 O1 -40.20(6) 3_345 2_365
O1 Ca1 Be1 O1 139.80(6) 9_565 2_365
O1 Ca1 Be1 O1 61.97(7) 8_445 2_365
O1 Ca1 Be1 O1 -118.03(7) 2_465 2_365
B4 Ca1 Be1 O1 -18.27(5) 1_455 2_365
B4 Ca1 Be1 O1 3.98(11) 7_465 2_365
B4 Ca1 Be1 O1 161.73(5) 7_455 2_365
B4 Ca1 Be1 O1 -176.02(11) 1_445 2_365
B4 Ca1 Be1 O1 -97.15(7) . 2_365
B4 Ca1 Be1 O1 82.85(7) 7_355 2_365
O1 Ca1 Be1 O1 -94.89(3) 7_355 3_235
O1 Ca1 Be1 O1 85.11(3) . 3_235
O1 Ca1 Be1 O1 -147.26(8) 3_345 3_235
O1 Ca1 Be1 O1 32.74(8) 9_565 3_235
O1 Ca1 Be1 O1 -45.10(6) 8_445 3_235
O1 Ca1 Be1 O1 134.90(6) 2_465 3_235
B4 Ca1 Be1 O1 -125.33(10) 1_455 3_235
B4 Ca1 Be1 O1 -103.09(6) 7_465 3_235
B4 Ca1 Be1 O1 54.67(10) 7_455 3_235
B4 Ca1 Be1 O1 76.91(6) 1_445 3_235
B4 Ca1 Be1 O1 155.79(6) . 3_235
B4 Ca1 Be1 O1 -24.21(6) 7_355 3_235
O1 Ca1 Be1 O1 180.0 7_355 .
O1 Ca1 Be1 O1 127.63(10) 3_345 .
O1 Ca1 Be1 O1 -52.37(10) 9_565 .
O1 Ca1 Be1 O1 -130.20(8) 8_445 .
O1 Ca1 Be1 O1 49.80(8) 2_465 .
B4 Ca1 Be1 O1 149.56(12) 1_455 .
B4 Ca1 Be1 O1 171.81(7) 7_465 .
B4 Ca1 Be1 O1 -30.44(12) 7_455 .
B4 Ca1 Be1 O1 -8.19(7) 1_445 .
B4 Ca1 Be1 O1 70.68(8) . .
B4 Ca1 Be1 O1 -109.32(8) 7_355 .
O1 Ca1 Be1 F1 109.32(8) 7_355 7_355
O1 Ca1 Be1 F1 -70.68(8) . 7_355
O1 Ca1 Be1 F1 56.95(3) 3_345 7_355
O1 Ca1 Be1 F1 -123.05(3) 9_565 7_355
O1 Ca1 Be1 F1 159.113(18) 8_445 7_355
O1 Ca1 Be1 F1 -20.887(18) 2_465 7_355
B4 Ca1 Be1 F1 78.88(6) 1_455 7_355
B4 Ca1 Be1 F1 101.12(6) 7_465 7_355
B4 Ca1 Be1 F1 -101.12(6) 7_455 7_355
B4 Ca1 Be1 F1 -78.88(6) 1_445 7_355
B4 Ca1 Be1 F1 0.0 . 7_355
B4 Ca1 Be1 F1 180.0 7_355 7_355
O1 Ca1 Be1 K1 33.40(14) 7_355 1_455
O1 Ca1 Be1 K1 -146.60(14) . 1_455
O1 Ca1 Be1 K1 -18.97(6) 3_345 1_455
O1 Ca1 Be1 K1 161.03(6) 9_565 1_455
O1 Ca1 Be1 K1 83.20(7) 8_445 1_455
O1 Ca1 Be1 K1 -96.80(7) 2_465 1_455
B4 Ca1 Be1 K1 2.96(5) 1_455 1_455
B4 Ca1 Be1 K1 25.21(12) 7_465 1_455
B4 Ca1 Be1 K1 -177.04(5) 7_455 1_455
B4 Ca1 Be1 K1 -154.79(12) 1_445 1_455
B4 Ca1 Be1 K1 -75.92(7) . 1_455
B4 Ca1 Be1 K1 104.08(7) 7_355 1_455
O1 Ca1 Be1 K1 -174.77(5) 7_355 1_445
O1 Ca1 Be1 K1 5.23(5) . 1_445
O1 Ca1 Be1 K1 132.87(9) 3_345 1_445
O1 Ca1 Be1 K1 -47.13(9) 9_565 1_445
O1 Ca1 Be1 K1 -124.97(8) 8_445 1_445
O1 Ca1 Be1 K1 55.03(8) 2_465 1_445
B4 Ca1 Be1 K1 154.79(12) 1_455 1_445
B4 Ca1 Be1 K1 177.04(5) 7_465 1_445
B4 Ca1 Be1 K1 -25.21(12) 7_455 1_445
B4 Ca1 Be1 K1 -2.96(5) 1_445 1_445
B4 Ca1 Be1 K1 75.92(7) . 1_445
B4 Ca1 Be1 K1 -104.08(7) 7_355 1_445
O1 Ca1 Be1 K1 109.32(8) 7_355 .
O1 Ca1 Be1 K1 -70.68(8) . .
O1 Ca1 Be1 K1 56.95(3) 3_345 .
O1 Ca1 Be1 K1 -123.05(3) 9_565 .
O1 Ca1 Be1 K1 159.113(18) 8_445 .
O1 Ca1 Be1 K1 -20.887(18) 2_465 .
B4 Ca1 Be1 K1 78.88(6) 1_455 .
B4 Ca1 Be1 K1 101.12(6) 7_465 .
B4 Ca1 Be1 K1 -101.12(6) 7_455 .
B4 Ca1 Be1 K1 -78.88(6) 1_445 .
B4 Ca1 Be1 K1 0.0 . .
B4 Ca1 Be1 K1 180.0 7_355 .
O1 Ca1 Be1 Ca1 -25.89(10) 7_355 1_455
O1 Ca1 Be1 Ca1 154.11(10) . 1_455
O1 Ca1 Be1 Ca1 -78.26(3) 3_345 1_455
O1 Ca1 Be1 Ca1 101.74(3) 9_565 1_455
O1 Ca1 Be1 Ca1 23.91(3) 8_445 1_455
O1 Ca1 Be1 Ca1 -156.09(3) 2_465 1_455
B4 Ca1 Be1 Ca1 -56.33(4) 1_455 1_455
B4 Ca1 Be1 Ca1 -34.08(8) 7_465 1_455
B4 Ca1 Be1 Ca1 123.67(4) 7_455 1_455
B4 Ca1 Be1 Ca1 145.92(8) 1_445 1_455
B4 Ca1 Be1 Ca1 -135.21(2) . 1_455
B4 Ca1 Be1 Ca1 44.79(2) 7_355 1_455
O1 Ca1 Be1 Ca1 -115.48(6) 7_355 1_445
O1 Ca1 Be1 Ca1 64.52(6) . 1_445
O1 Ca1 Be1 Ca1 -167.84(4) 3_345 1_445
O1 Ca1 Be1 Ca1 12.16(4) 9_565 1_445
O1 Ca1 Be1 Ca1 -65.68(3) 8_445 1_445
O1 Ca1 Be1 Ca1 114.32(3) 2_465 1_445
B4 Ca1 Be1 Ca1 -145.92(7) 1_455 1_445
B4 Ca1 Be1 Ca1 -123.67(4) 7_465 1_445
B4 Ca1 Be1 Ca1 34.08(7) 7_455 1_445
B4 Ca1 Be1 Ca1 56.33(4) 1_445 1_445
B4 Ca1 Be1 Ca1 135.21(2) . 1_445
B4 Ca1 Be1 Ca1 -44.79(2) 7_355 1_445
O1 Ca1 B4 O1 65.13(13) 7_355 3_445
O1 Ca1 B4 O1 -114.87(13) . 3_445
O1 Ca1 B4 O1 166.61(14) 3_345 3_445
O1 Ca1 B4 O1 -13.39(14) 9_565 3_445
O1 Ca1 B4 O1 97.52(5) 8_445 3_445
O1 Ca1 B4 O1 -82.48(5) 2_465 3_445
B4 Ca1 B4 O1 170.19(10) 1_455 3_445
B4 Ca1 B4 O1 89.20(16) 7_465 3_445
B4 Ca1 B4 O1 -9.81(10) 7_455 3_445
B4 Ca1 B4 O1 -90.80(16) 1_445 3_445
B4 Ca1 B4 O1 -42.78(11) 7_355 3_445
O1 Ca1 B4 O1 147.61(8) 7_355 2_465
O1 Ca1 B4 O1 -32.39(8) . 2_465
O1 Ca1 B4 O1 -110.92(10) 3_345 2_465
O1 Ca1 B4 O1 69.08(10) 9_565 2_465
O1 Ca1 B4 O1 180.0 8_445 2_465
B4 Ca1 B4 O1 -107.33(6) 1_455 2_465
B4 Ca1 B4 O1 171.67(11) 7_465 2_465
B4 Ca1 B4 O1 72.67(6) 7_455 2_465
B4 Ca1 B4 O1 -8.33(11) 1_445 2_465
B4 Ca1 B4 O1 39.70(7) 7_355 2_465
O1 Ca1 B4 O1 -67.40(8) 7_355 1_665
O1 Ca1 B4 O1 112.60(8) . 1_665
O1 Ca1 B4 O1 34.07(8) 3_345 1_665
O1 Ca1 B4 O1 -145.93(8) 9_565 1_665
O1 Ca1 B4 O1 -35.01(16) 8_445 1_665
O1 Ca1 B4 O1 144.99(16) 2_465 1_665
B4 Ca1 B4 O1 37.65(11) 1_455 1_665
B4 Ca1 B4 O1 -43.34(6) 7_465 1_665
B4 Ca1 B4 O1 -142.35(11) 7_455 1_665
B4 Ca1 B4 O1 136.66(6) 1_445 1_665
B4 Ca1 B4 O1 -175.32(10) 7_355 1_665
O1 Ca1 B4 Ca1 -24.06(3) 7_355 1_665
O1 Ca1 B4 Ca1 155.94(3) . 1_665
O1 Ca1 B4 Ca1 77.41(3) 3_345 1_665
O1 Ca1 B4 Ca1 -102.59(3) 9_565 1_665
O1 Ca1 B4 Ca1 8.33(11) 8_445 1_665
O1 Ca1 B4 Ca1 -171.67(11) 2_465 1_665
B4 Ca1 B4 Ca1 80.99(6) 1_455 1_665
B4 Ca1 B4 Ca1 0.0 7_465 1_665
B4 Ca1 B4 Ca1 -99.01(6) 7_455 1_665
B4 Ca1 B4 Ca1 180.0 1_445 1_665
B4 Ca1 B4 Ca1 -131.98(5) 7_355 1_665
O1 Ca1 B4 Ca1 74.94(4) 7_355 1_655
O1 Ca1 B4 Ca1 -105.06(4) . 1_655
O1 Ca1 B4 Ca1 176.42(4) 3_345 1_655
O1 Ca1 B4 Ca1 -3.58(4) 9_565 1_655
O1 Ca1 B4 Ca1 107.33(6) 8_445 1_655
O1 Ca1 B4 Ca1 -72.67(6) 2_465 1_655
B4 Ca1 B4 Ca1 180.0 1_455 1_655
B4 Ca1 B4 Ca1 99.01(6) 7_465 1_655
B4 Ca1 B4 Ca1 0.0 7_455 1_655
B4 Ca1 B4 Ca1 -80.99(6) 1_445 1_655
B4 Ca1 B4 Ca1 -32.971(18) 7_355 1_655
O1 Ca1 B4 K1 -154.559(19) 7_355 .
O1 Ca1 B4 K1 25.441(19) . .
O1 Ca1 B4 K1 -53.09(2) 3_345 .
O1 Ca1 B4 K1 126.91(2) 9_565 .
O1 Ca1 B4 K1 -122.17(8) 8_445 .
O1 Ca1 B4 K1 57.83(8) 2_465 .
B4 Ca1 B4 K1 -49.50(3) 1_455 .
B4 Ca1 B4 K1 -130.50(3) 7_465 .
B4 Ca1 B4 K1 130.50(3) 7_455 .
B4 Ca1 B4 K1 49.50(3) 1_445 .
B4 Ca1 B4 K1 97.526(14) 7_355 .
O1 Ca1 B4 K1 141.62(7) 7_355 1_655
O1 Ca1 B4 K1 -38.38(7) . 1_655
O1 Ca1 B4 K1 -116.91(8) 3_345 1_655
O1 Ca1 B4 K1 63.09(8) 9_565 1_655
O1 Ca1 B4 K1 174.00(5) 8_445 1_655
O1 Ca1 B4 K1 -6.00(5) 2_465 1_655
B4 Ca1 B4 K1 -113.33(4) 1_455 1_655
B4 Ca1 B4 K1 165.68(9) 7_465 1_655
B4 Ca1 B4 K1 66.67(4) 7_455 1_655
B4 Ca1 B4 K1 -14.32(9) 1_445 1_655
B4 Ca1 B4 K1 33.70(5) 7_355 1_655
O1 Ca1 B4 K1 -90.73(6) 7_355 1_665
O1 Ca1 B4 K1 89.27(6) . 1_665
O1 Ca1 B4 K1 10.74(6) 3_345 1_665
O1 Ca1 B4 K1 -169.26(6) 9_565 1_665
O1 Ca1 B4 K1 -58.35(14) 8_445 1_665
O1 Ca1 B4 K1 121.65(14) 2_465 1_665
B4 Ca1 B4 K1 14.32(9) 1_455 1_665
B4 Ca1 B4 K1 -66.67(4) 7_465 1_665
B4 Ca1 B4 K1 -165.68(9) 7_455 1_665
B4 Ca1 B4 K1 113.33(4) 1_445 1_665
B4 Ca1 B4 K1 161.35(8) 7_355 1_665
F1 K1 B4 O1 35.49(8) 7_455 3_445
F1 K1 B4 O1 -105.62(10) 7_465 3_445
F1 K1 B4 O1 144.93(9) 7_355 3_445
O1 K1 B4 O1 -168.65(11) 3_345 3_445
O1 K1 B4 O1 -88.20(4) 5_564 3_445
O1 K1 B4 O1 94.44(3) 2_465 3_445
O1 K1 B4 O1 13.23(11) 6_354 3_445
O1 K1 B4 O1 124.22(9) . 3_445
O1 K1 B4 O1 -52.38(9) 4_444 3_445
Be1 K1 B4 O1 -137.34(13) 1_665 3_445
Be1 K1 B4 O1 144.93(9) 4_334 3_445
Be1 K1 B4 O1 12.21(10) 4_434 3_445
F1 K1 B4 O1 -58.95(6) 7_455 2_465
F1 K1 B4 O1 159.94(8) 7_465 2_465
F1 K1 B4 O1 50.50(7) 7_355 2_465
O1 K1 B4 O1 96.91(9) 3_345 2_465
O1 K1 B4 O1 177.36(2) 5_564 2_465
O1 K1 B4 O1 -81.21(9) 6_354 2_465
O1 K1 B4 O1 29.78(7) . 2_465
O1 K1 B4 O1 -146.82(6) 4_444 2_465
Be1 K1 B4 O1 128.22(11) 1_665 2_465
Be1 K1 B4 O1 50.50(7) 4_334 2_465
Be1 K1 B4 O1 -82.23(8) 4_434 2_465
F1 K1 B4 O1 165.62(9) 7_455 1_665
F1 K1 B4 O1 24.51(7) 7_465 1_665
F1 K1 B4 O1 -84.94(8) 7_355 1_665
O1 K1 B4 O1 -38.52(7) 3_345 1_665
O1 K1 B4 O1 41.93(13) 5_564 1_665
O1 K1 B4 O1 -135.43(13) 2_465 1_665
O1 K1 B4 O1 143.36(7) 6_354 1_665
O1 K1 B4 O1 -105.65(8) . 1_665
O1 K1 B4 O1 77.75(8) 4_444 1_665
Be1 K1 B4 O1 -7.21(6) 1_665 1_665
Be1 K1 B4 O1 -84.94(8) 4_334 1_665
Be1 K1 B4 O1 142.34(8) 4_434 1_665
F1 K1 B4 Ca1 169.92(8) 7_455 1_665
F1 K1 B4 Ca1 28.80(5) 7_465 1_665
F1 K1 B4 Ca1 -80.64(7) 7_355 1_665
O1 K1 B4 Ca1 -34.22(6) 3_345 1_665
O1 K1 B4 Ca1 46.22(12) 5_564 1_665
O1 K1 B4 Ca1 -131.13(13) 2_465 1_665
O1 K1 B4 Ca1 147.66(6) 6_354 1_665
O1 K1 B4 Ca1 -101.36(7) . 1_665
O1 K1 B4 Ca1 82.05(7) 4_444 1_665
Be1 K1 B4 Ca1 -2.92(5) 1_665 1_665
Be1 K1 B4 Ca1 -80.64(7) 4_334 1_665
Be1 K1 B4 Ca1 146.64(6) 4_434 1_665
F1 K1 B4 Ca1 -28.80(5) 7_455 1_655
F1 K1 B4 Ca1 -169.92(8) 7_465 1_655
F1 K1 B4 Ca1 80.64(7) 7_355 1_655
O1 K1 B4 Ca1 127.05(8) 3_345 1_655
O1 K1 B4 Ca1 -152.50(4) 5_564 1_655
O1 K1 B4 Ca1 30.14(5) 2_465 1_655
O1 K1 B4 Ca1 -51.06(8) 6_354 1_655
O1 K1 B4 Ca1 59.92(7) . 1_655
O1 K1 B4 Ca1 -116.67(7) 4_444 1_655
Be1 K1 B4 Ca1 158.36(11) 1_665 1_655
Be1 K1 B4 Ca1 80.64(7) 4_334 1_655
Be1 K1 B4 Ca1 -52.09(8) 4_434 1_655
F1 K1 B4 Ca1 -109.442(13) 7_455 .
F1 K1 B4 Ca1 109.442(13) 7_465 .
F1 K1 B4 Ca1 0.0 7_355 .
O1 K1 B4 Ca1 46.41(2) 3_345 .
O1 K1 B4 Ca1 126.86(6) 5_564 .
O1 K1 B4 Ca1 -50.50(7) 2_465 .
O1 K1 B4 Ca1 -131.70(2) 6_354 .
O1 K1 B4 Ca1 -20.717(15) . .
O1 K1 B4 Ca1 162.687(15) 4_444 .
Be1 K1 B4 Ca1 77.72(6) 1_665 .
Be1 K1 B4 Ca1 0.0 4_334 .
Be1 K1 B4 Ca1 -132.73(3) 4_434 .
F1 K1 B4 K1 27.198(8) 7_455 1_655
F1 K1 B4 K1 -113.92(3) 7_465 1_655
F1 K1 B4 K1 136.64(2) 7_355 1_655
O1 K1 B4 K1 -176.94(3) 3_345 1_655
O1 K1 B4 K1 -96.50(5) 5_564 1_655
O1 K1 B4 K1 86.14(6) 2_465 1_655
O1 K1 B4 K1 4.94(4) 6_354 1_655
O1 K1 B4 K1 115.92(3) . 1_655
O1 K1 B4 K1 -60.67(3) 4_444 1_655
Be1 K1 B4 K1 -145.64(7) 1_665 1_655
Be1 K1 B4 K1 136.64(2) 4_334 1_655
Be1 K1 B4 K1 3.91(4) 4_434 1_655
F1 K1 B4 K1 113.92(3) 7_455 1_665
F1 K1 B4 K1 -27.198(7) 7_465 1_665
F1 K1 B4 K1 -136.64(2) 7_355 1_665
O1 K1 B4 K1 -90.23(3) 3_345 1_665
O1 K1 B4 K1 -9.78(8) 5_564 1_665
O1 K1 B4 K1 172.86(8) 2_465 1_665
O1 K1 B4 K1 91.66(3) 6_354 1_665
O1 K1 B4 K1 -157.36(2) . 1_665
O1 K1 B4 K1 26.05(2) 4_444 1_665
Be1 K1 B4 K1 -58.92(5) 1_665 1_665
Be1 K1 B4 K1 -136.64(2) 4_334 1_665
Be1 K1 B4 K1 90.63(3) 4_434 1_665
O1 Be1 O1 B4 172.31(14) 2_365 1_445
O1 Be1 O1 B4 41.4(2) 3_235 1_445
F1 Be1 O1 B4 -73.14(14) 7_355 1_445
K1 Be1 O1 B4 -117.4(2) 1_455 1_445
K1 Be1 O1 B4 -16.44(16) 1_445 1_445
K1 Be1 O1 B4 -111.63(15) . 1_445
Ca1 Be1 O1 B4 127.09(13) 1_455 1_445
Ca1 Be1 O1 B4 159.60(17) . 1_445
Ca1 Be1 O1 B4 50.05(15) 1_445 1_445
O1 Be1 O1 Ca1 12.70(16) 2_365 .
O1 Be1 O1 Ca1 -118.19(9) 3_235 .
F1 Be1 O1 Ca1 127.26(4) 7_355 .
K1 Be1 O1 Ca1 83.0(2) 1_455 .
K1 Be1 O1 Ca1 -176.04(4) 1_445 .
K1 Be1 O1 Ca1 88.77(5) . .
Ca1 Be1 O1 Ca1 -32.51(9) 1_455 .
Ca1 Be1 O1 Ca1 -109.55(5) 1_445 .
O1 Be1 O1 K1 -76.07(13) 2_365 .
O1 Be1 O1 K1 153.04(12) 3_235 .
F1 Be1 O1 K1 38.49(3) 7_355 .
K1 Be1 O1 K1 -5.7(2) 1_455 .
K1 Be1 O1 K1 95.19(4) 1_445 .
Ca1 Be1 O1 K1 -121.28(4) 1_455 .
Ca1 Be1 O1 K1 -88.77(5) . .
Ca1 Be1 O1 K1 161.68(3) 1_445 .
O1 Ca1 O1 B4 4.80(13) 7_355 1_445
O1 Ca1 O1 B4 148.48(8) 3_345 1_445
O1 Ca1 O1 B4 -31.52(8) 9_565 1_445
O1 Ca1 O1 B4 -115.57(9) 8_445 1_445
O1 Ca1 O1 B4 64.43(9) 2_465 1_445
B4 Ca1 O1 B4 171.40(11) 1_455 1_445
B4 Ca1 O1 B4 180.0 7_465 1_445
B4 Ca1 O1 B4 -8.60(11) 7_455 1_445
B4 Ca1 O1 B4 77.33(7) . 1_445
B4 Ca1 O1 B4 -102.67(7) 7_355 1_445
O1 Ca1 O1 Be1 169.48(11) 7_355 .
O1 Ca1 O1 Be1 -46.84(9) 3_345 .
O1 Ca1 O1 Be1 133.16(9) 9_565 .
O1 Ca1 O1 Be1 49.10(8) 8_445 .
O1 Ca1 O1 Be1 -130.90(8) 2_465 .
B4 Ca1 O1 Be1 -23.93(9) 1_455 .
B4 Ca1 O1 Be1 -15.33(12) 7_465 .
B4 Ca1 O1 Be1 156.07(9) 7_455 .
B4 Ca1 O1 Be1 164.67(12) 1_445 .
B4 Ca1 O1 Be1 -118.00(8) . .
B4 Ca1 O1 Be1 62.00(8) 7_355 .
O1 Ca1 O1 K1 -102(91) 7_355 .
O1 Ca1 O1 K1 42.027(14) 3_345 .
O1 Ca1 O1 K1 -137.973(14) 9_565 .
O1 Ca1 O1 K1 137.973(14) 8_445 .
O1 Ca1 O1 K1 -42.027(14) 2_465 .
B4 Ca1 O1 K1 64.94(3) 1_455 .
B4 Ca1 O1 K1 73.54(9) 7_465 .
B4 Ca1 O1 K1 -115.06(3) 7_455 .
B4 Ca1 O1 K1 -106.46(9) 1_445 .
B4 Ca1 O1 K1 -29.13(2) . .
B4 Ca1 O1 K1 150.87(2) 7_355 .
F1 K1 O1 B4 -18.37(7) 7_455 1_445
F1 K1 O1 B4 -144.61(7) 7_465 1_445
F1 K1 O1 B4 109.88(7) 7_355 1_445
O1 K1 O1 B4 -147.82(7) 3_345 1_445
O1 K1 O1 B4 109.88(7) 5_564 1_445
O1 K1 O1 B4 -73.24(8) 2_465 1_445
O1 K1 O1 B4 35.39(7) 6_354 1_445
O1 K1 O1 B4 -18.37(7) 4_444 1_445
Be1 K1 O1 B4 -133.41(7) 1_665 1_445
Be1 K1 O1 B4 96.92(7) 4_334 1_445
Be1 K1 O1 B4 3.47(7) 4_434 1_445
F1 K1 O1 Be1 -154.87(6) 7_455 .
F1 K1 O1 Be1 78.89(6) 7_465 .
F1 K1 O1 Be1 -26.62(6) 7_355 .
O1 K1 O1 Be1 75.68(7) 3_345 .
O1 K1 O1 Be1 -26.62(6) 5_564 .
O1 K1 O1 Be1 150.26(6) 2_465 .
O1 K1 O1 Be1 -101.11(6) 6_354 .
O1 K1 O1 Be1 -154.87(6) 4_444 .
Be1 K1 O1 Be1 90.10(5) 1_665 .
Be1 K1 O1 Be1 -39.58(7) 4_334 .
Be1 K1 O1 Be1 -133.02(3) 4_434 .
F1 K1 O1 Ca1 92.156(16) 7_455 .
F1 K1 O1 Ca1 -34.08(3) 7_465 .
F1 K1 O1 Ca1 -139.59(2) 7_355 .
O1 K1 O1 Ca1 -37.287(9) 3_345 .
O1 K1 O1 Ca1 -139.59(2) 5_564 .
O1 K1 O1 Ca1 37.287(9) 2_465 .
O1 K1 O1 Ca1 145.92(3) 6_354 .
O1 K1 O1 Ca1 92.156(16) 4_444 .
Be1 K1 O1 Ca1 -22.88(2) 1_665 .
Be1 K1 O1 Ca1 -152.55(2) 4_334 .
Be1 K1 O1 Ca1 114.00(3) 4_434 .
